topical workshop on Anti e-Cloud Coatings “AEC'09” http://indico.cern.ch/conferenceDisplay.py?confId=62873 organized by EuCARD-AccNet-EuroLumi and SPS Upgrade Study Team http://eucard.web.cern.ch/EuCARD/index.html http://accnet.lal.in2p3.fr/ http://paf-spsu.web.cern.ch/paf-spsu/
Summary, by M.Taborelli (CERN-TE-VSC) TiN SNS findings (M.Plum, Oak Ridge), TiN in J-Parc (S.Kato), TiN at KEK (Shibata), TiN in CESR-TA (M.Palmer, Cornell), TiN at SLAC(M.Pivi) Carbon coatings Characterization (M.Taborelli, CERN), SPS e-cloud CESR-TA(C.Yin-Vallgren, CERN), SPS pressure (M.Taborelli, CERN), SPS dipole coating, technique (P.Costa Pinto,CERN), SPS coating, strategy for the entire machine (J.Bauche, CERN), Impedance (D.Seebacher,CERN), Microwave diagnostics (F.Caspers, CERN), DLC (S.Kato, KEK) Low SEY by rough surfaces and grooves Rough surfaces (I.Montero, CSIC Madrid) Grooves (M.Pivi), Grooves with TiN (M.Palmer, Cornell) Clearing electrodes (E.Mahner, CERN) Simulations: SPS situation (G.Rumolo CERN), CESR-TA situation (J.Crittenden, Cornell) My comments are in red …and I tried to be honest!
TiN coatings • SNS (M.Plum, Oak Ridge): protons • 95% of the accumulator ring is coated with TiN, 100nm thick, SEY not measured, conditioning state uncertain • there is e-p instability in the ring at 1/5 of nominal intensity (3E13p/b), it was not predicted by simulations including TiN coating as well as for those considering StSt surfaces ( =2) • Ring-RF can control the instability • is TiN really useful? Effectiveness should be verified Vertical Horizontal
TiN coatings • TiN in J-Parc (S.Kato, KEK): protons • -on alumina chambers used in RCS (rapid cycling synchrotron) magnets (200m coated chambers on 350m machine), 15 nm thick coating, by hollow cathode technique • -no problems after 1 year of operation, however at very low beam intensity, not in e-cloud conditions • no evidence of e-cloud in the ring (pressure monitoring) • very low static degassing (better than unbaked StSt) • no direct measurement of SEY, guess 0.8-1.1 after conditioning Probably on alumina almost everything would lower the SEY: how low SEY is needed?
TiN coatings TiN in CESR-TA (M.Palmer, Cornell): e+,e- • RFA signal (e-cloud) in drift space: photons from dipole! • TiN as Cu, for e+ beam (where also e-cloud is expected) • TiN better than Cu for e- beam (where no e-cloud is expected and the signal is dominated by photoelectrons) • conditioned TiN seems good with photons (low photoyield?) e+ e- Cu TiN Cu TiN
TiN coatings VP4031 (6-8)-Jul-01 Solenoid OFF TiN in PEPII-LER (M.Pivi, SLAC): e+ -e-cloud in uncoated StSt straight sections (pressure rise) -no e-cloud in TiN coated arcs Arcs TiN coated Straight sections uncoated Beam current Beam current • PEP-II reached 3 x Design Peak Luminosity. Presumably TiN coating and antechamber in arcs played a big role (!) • No direct data about TiN coated vs un-coated, since no electron detectors were installed at the time yet, i.e. 2003. • Note also larger chamber aperture in straight sections
TiN coatings Removable samples exposed to the beam environment and measured in the lab after conditioning by the PEPII beam: • TiN best performances, measured SEY < 1, • Carbon and Oxygen content decreased • Kept in stand-by in vacuum: SEY<1 even after 1000 hours (!) • Aluminum conditioned but still SEY > 2! Conditioning through photons (and ions? how much?). Note that conditioning with e-beam in the lab gives increasing C (S.Kato)
TiN coatings K.Shibata (KEK): LER (Super)KEKB, e+ -Producing TiN/Cu: best samples for adhesion on Cu and low SEY (max= 1.2 at 1E-5C/mm2) on 150C substrate -Unbaked coated pipe has 5 times more outgassing than Cu uncoated pipe, but moderate baking (80-100C) can lower outgassing to the level of uncoated Cu chamber -lower e-cloud than in uncoated chamber In KEK LER Copper Again TiN is good with photons! In conditioned state K. Kanazawa TiN-coated duct (94 mm) TiN (KEK) TiN (BNL) In the following autumn run, Al ducts and groove surfaces (Al and Cu) with and without the TiN coating will be tested in KEKB LER
TiN coatings TiN measurements in the lab: (S.Kato, KEK) As received state Dose of irradiation in the lab at 5KeV electrons Data consistent with other labs (CERN, SLAC) After a strong conditioning by an e-beam almost everything is good
C coatings SEY of carbon a-C coatings (M.Taborelli) accuracy +/-0.03 -no bake-out -as expected SEY does not change for thicknesses above 50 nm -scattering in production 0.9< δmax <1.1 -aging is moderate in N2, dessicator or wrapped in Al foil -partial recovery possible by heating (200C ) or plasma cleaning
C coatings a-C coatings results from e-cloud monitors in SPS (C.Yin-Vallgren) LHC type beam at 25ns spacing, 72 bunches, 1-3 batches Strong reduction of e-cloud current a-C(2 month in SPS) 0 0 a-C(1.33) -1E-4 a-C(0.92) -1 StSt (2.5) -2E-4 E-cloud current/FBCT a-C(1.14) -3E-4 -2 -4E-4 0 1 2 3 4 5 Time(SPS Cycles) Time(h)
C coatings Impedance of the coatings (D.Seebacher) • Cavity perturbation (detuning) method was used to measure the properties (2-4GHz range) • Coatings of NEG and a-C of different thickness on glass rods, inserted in the cavity • NEG shows resistive behaviour (metallic conductor); conductivity is too high to be measured • a-C shows the behaviour of a bad conductor (4000S/m, 0.25mthick, or 1k square) with no effect of dielectric constant Strange behaviour as a function of frequency: the rod is not a small perturbation!
C coatings Coating of 3 MMB dipoles for SPS tests (P.Costa Pinto) DESIGN and BUILT-UP January 2009: arrival of first pieces: assemble vacuum and bench. February 2009: adapt electrodes. Start tests and coatings. March 2009: insertion in SPS
C coatings Pressure measurements in SPS (M.Taborelli) a-C coated dipoles uncoated dipoles 12 3 4 batches x 72 bunches at 90% of nominal intensity, 450GeV Time[hh:mm:ss] Pressure rise is stronger between 1st and 2nd; coated magnets are only slightly better for higher number of batches. Less improvement than expected.
C coatings Example of previously inspected quad (courtesy of K.Cornelis) E.Mahner E-cloud in uncoated areas E-cloud occurs in these areas too! The RF-shields show discoloration lines (inspection 6/10/2009) Colored lines are present also in the quadrupole close to the coated MBB Region of RF shields (uncoated) close to the pressure gauge and pumping port We replaced the shields with a-C coated shields and will measure again
C coatings S. Federmann • Measurement of phase modulation of a microwave (MW) signal due to ecloud, in principle sensitive to the e-cloud density where it travels Beam 1 batch, 72 bunches: PM signal in uncoated magnet 10 dB above noise Coated magnets Uncoated magnets Next test at 75 ns It is difficult, it is not well understood yet but it is worth to be continued since it is a direct measurement of what happens in the dipoles! 1-2-3 batches 16
C coatings Comparison Al, a-C/Al, Cu, TiN/Cu at CESRTA (S.Calatroni) CESR-TA results on a-C CERN coated chamber: conditioned state e+ e- Al Al Cu Cu TiN a-C TiN a-C • a-C is much better than bare Al and better Cu for both, e+ and e- • -TiN is better for “only photons”, a-C is better when e-cloud might occur • -possible corrections could come from photon flux differences (local machine geometry) • -a-C chamber contaminated with silicone (kapton adhesive tape) during acceptance test
C coatings Graphitization and DLC coatings: (S.Kato, KEK) -Conditioing with e-beam induces an increase of C on the surface and decreases SEY -Graphitic C…called graphitization: try to do it on the beampipe before insertion by bombarding with electrons from a filament -Compare with DLC coating (commercial) KEKB: e-cloud monitor in the machine • Conditioned state • Graphitization layer is probably too thin • DLC is not considered of the best quality which can be achieved: the experiment will be repeated this fall with a better coating
RFA collectors are tricky! -Transmission should be simulated and taken into account for interpretation of the data: depends on B-field (see e-cloud monitors in SPS), on angle of incidence of the electrons….. -Energy spectrum of the collected electrons is even very difficult to measure due to secondary electrons generated in the RFA itself and angular effects -Design of all collectors seen is much more primitive that all what is done in surface science analysis systems, due “accelerator constraints (space, integration in a vacuum chamber, surrounding noise ……) -Materials used are often at the edge of compatibility with UHV
C-Coatings Logistics for SPS dipole coating campaign: (J.Bauche) • Three possible strategies • Cleaning/coating in the SPS tunnel • Cleaning/coating in ECX5 cavern • Cleaning/coating on surface • Obvious differences in radiation levels to cope with, transport (more or less handling is needed, handling of waste……the best solution must still bed ecided by putting everything on the balance • In all cases 3 shutdown periods are necessary • -All should be in place for 2015 typically
Other projects for coatings against e-cloud: FNAL (U,Wienands), TiN for upgrade of main injector of project X The setup will be assembled in the next few weeks (short prototype); needs articulated electrode to coat dipoles (1.5 cm sagitta), by magnetron (SLAC technique) Coupons will be used to monitor thickness, nominal value is 100 nm Coating is expected for November. Coating in situ (A.Herskovitch, BNL) with a mole RHIC for electrons Would like to coat 500m in situ Very preliminary stage of the study Not decided which coating
Simulations (G.Rumolo) (the MBB threshold is max<1.3) (including chamber edges with fringe fields)
Rough surfaces 2.5 2.0 1.5 SEE coeficient Ag plated 1.0 E1 chem. etched 0.5 Au coated Au / c-Si 0.0 0 200 400 600 800 1000 1200 1400 Primary Electron Energy [eV] Lowering SEY by rough surfaces (I.Montero, CSIC Madrid) Microstructured Au coating The surface is fragile! Issues for degassing if it cannot be baked (resistance to temperature treatment not verified)
AEC’09 I. Montero CERN 12.10.09 Metallic/Dielectric Microparticles Coatings Extreme reduction of SEY Al particle Al2O3 particle Gold coated Surface top view
grooves E-cloud suppression with grooves (M.Pivi, SLAC) E-cloud detection in straight section of PEPII Flat surface grooves Al extrusion +TiN coating
…and in a dipole (M.Palmer, M.Pivi) grooves • Current scan in L3 Chicane, 1x45 e+, 14ns, 5GeV (chicane of SLAC to Cornell • Note: Al signal is divided by 20 to show on the same scale • Grooved chamber has 5mm deep 20° triangular grooves with TiN coating Bare Al (1/20) No grooves grooves M. Palmer Cornell